Abstract
A longstanding issue in topological insulator research has been to find a bulk single crystal material that provides a highquality platform for characterizing topological surface states without interference from bulk electronic states. This material would ideally be a bulk insulator, have a surface state Dirac point energy well isolated from the bulk valence and conduction bands, display quantum oscillations from the surface state electrons and be growable as large, highquality bulk single crystals. Here we show that this material obstacle is overcome by bulk crystals of lightly Sndoped Bi_{1.1}Sb_{0.9}Te_{2}S grown by the vertical Bridgman method. We characterize SnBSTS via angleresolved photoemission spectroscopy, scanning tunnelling microscopy, transport studies, Xray diffraction and Raman scattering. We present this material as a highquality topological insulator that can be reliably grown as bulk single crystals and thus studied by many researchers interested in topological surface states.
Introduction
Topological insulators (TIs) display a new state of quantum matter^{1,2,3,4,5}. In these threedimensional, small band gap bulk insulators, metallic twodimensional spinmomentum locked Dirac fermions exist on the surfaces. These fermions, exhibiting a quasilinear energy versus wavevector dispersion relation near their Dirac point (DP), owe their existence and protection to the timereversal symmetry^{6}. Threedimensional TIs have sparked wide interest in the research community due to both their fundamental scientific interest and the opportunities they offer for observing new electronic phenomena and properties that may be exploited for spintronics or other advanced electronic applications^{7,8,9,10,11,12,13}. Unfortunately, however, the transport properties of the actual materials involved are typically dominated by the bulk electrons^{5,14,15,16}, making the true electronic properties of the surface states (SSs) difficult to observe and exploit.
Bi_{2}Se_{3} and Bi_{2}Te_{3}, with bulk band gaps of ∼300 and ∼150 meV, respectively, are members of the larger M_{2}X_{3} (M=Sb, Bi; X=S, Se, Te) tetradymite family and are widely considered to be fundamental materials platforms for the investigation of topological SSs (TSSs). The best bulk Bi_{2}Se_{3} crystals are heavily doped^{16}, with their Fermi level in the bulk conduction band (BCB), and thus the SS cannot be characterized independently of interference from the bulk states and in Bi_{2}Te_{3} the SS DP energy is below that of the top of the bulk valence band (BVB) and the crystals have large bulk carrier concentrations due to antisite defects^{17,18}. Thus, neither of the simple materials is suitable for experimentally probing the intrinsic character of the TSS.
Efforts have been underway since the inception of the field, to find a material that is the best bulk single crystal TI for studying the intrinsic properties of the surface Dirac electrons^{19,20,21,22,23,24,25,26,27,28,29,30}. So far, the primary desirable characteristics for the ideal bulk crystal material—to have a SS DP well isolated in energy from the bulk states and a very low bulk carrier concentration, both of which would allow for the study of the Dirac electrons at very low energies without interference from the bulk states, quantum oscillations from the TSS electrons and reliable growability as highquality single crystals—have proven to be difficult, to satisfy in a single real bulk material. Until the current work, Bi_{2}Te_{2}Se, with wellcontrolled stoichiometry and defect chemistry, has been considered as the best bulk crystal material from this perspective, but its DP energy is below the maximum energy of the BVB by ∼60 meV, making it impossible to study the SS electrons close to the DP without interference from bulk states^{20,24,25,26,27}. An alternative material is the quaternary solid solution (Bi_{1−x}Sb_{x})_{2}(Se_{1−y}Te_{y})_{3} (refs 28, 29, 30), but the stoichiometry of that material is not fixed by any intrinsic thermodynamic material characteristic such as chemistry or structure, making it unsuitable as a general materials platform for the study of TSS. Although very important measurements have been performed on carefully prepared thin films of materials in the (Bi_{1−x}Sb_{x})_{2}(Se_{1−y}Te_{y})_{3} family, the lack of a bulk material with excellent properties that can be reproducibly grown as large bulk single crystals has significantly limited the number of experimental research groups that can contribute to the development of the field.
Here we describe the design, growth and characterization of a material that we argue satisfies all the synthesis and electronic structure criteria to be an ideal bulk TI. This material is derived by combining concepts in crystal chemistry, defect chemistry, strainmediated chemical stability, the effect of atomic electronegativities on the absolute energies of bulk electronic states and resonant level doping. The result is the stable, bulkinsulating, highcrystallinity single crystal material Bi_{1.1}Sb_{0.9}Te_{2}S, grown by the vertical Bridgman technique (VBT) and doped with a very small percentage of Sn. Large crystals with excellent properties can be reproducibly grown. This material displays an SS DP energy fully isolated from the BVB and BCB, verylow bulk carrier concentrations, strong domination of the conductance by surface currents below 100 K and reproducibly observed quantum oscillations from the TSSs. Its growth, described here, will make the characterization of TSSs available to a wide community of researchers.
Results
Material design
Figure 1a shows a schematic view of the materials design process that leads us to Bi_{1.08}Sn_{0.02}Sb_{0.9}Te_{2}S (SnBSTS). We start with Bi_{2}Se_{3} and Bi_{2}Te_{3}, which are the simplest, although far from ideal, tetradymitetype TI materials. To obtain bulk insulating TI crystals based on these tetradymites, two main approaches and their combination have been employed. In Approach1, starting from Bi_{2}Se_{3}, Te has been partially substituted for Se to form Bi_{2}Te_{2}Se (BTS), where the electrondonating Se vacancies in Bi_{2}Se_{3} are controlled by confining the Se to the middle layer in the quintuplelayer (QL) structure or, alternatively, by the much less wellcontrolled random Bi_{2}(Se_{1−x}Te_{x})_{3} solid solution. In Approach2, the composition of Bisite is adjusted by SbBi partial substitution. This method has the advantage of yielding materials, whose DP is isolated from the bulk states, but the defect chemistry is again difficult to control. By using both approaches simultaneously, yielding tetradymites of the type (Bi_{1−x}Sb_{x})_{2}(Se_{1−y}Te_{y})_{3}, the energy of the SS DP can be placed in the bulk band gap, and films and crystals can be grown with low bulk carrier concentrations at low temperature^{28,29,30}. The disadvantage of this material is the difficulty in controlling its composition and therefore its defect chemistry, to grow large highquality bulk single crystals.
Here we develop an alternative material system based on incorporating S rather than Se in the middle layer of Bi_{2}Te_{2}Se. The incorporation of S in place of Se in the middle layer of the tetradymite QL sandwich decreases the absolute energy of the valence band due to the higher electronegativity^{31} of S and makes the surface DP isolated in energy from the bulk states. This is a parallel materials development path to Approach1. However, the formation of a thermodynamically stable compound of composition Bi_{2}Te_{2}S is not possible, due to crystallographic strain from layer size mismatch, as was early described by Pauling^{32} and so a decrease of the size of the Bi layers must be made through Approach2 to obtain a stable material. Through experimentation we have found that the composition of that stable material is Bi_{1.1}Sb_{0.9}Te_{2}S. This composition is a result of chemical synergism: the incorporation of S in the middle of the QL requires a contraction of the metal layers (the ones containing Bi and Sb, Sb is smaller than Bi) for size matching and selects a Bi/Sb ratio near 1:1 for stability (Fig. 1b). This is a very strong crystalchemical driving force for stability and results in the optimal growth of this composition as large single crystals directly from a melt of the same composition. This material already has a low carrier concentration, but as a final step we employ the concept of resonant level doping, developed in previous work to optimize the properties of tetradymite thermoelectrics, where small amounts of Sn are known to act in that capacity^{24,25,33}, to compensate for the last of the native defects present. We thus obtain a bulkinsulating ideal TI through 1% Sn substitution for Bi and Sb and develop the material Bi_{1.08}Sn_{0}._{02}Sb_{0.9}Te_{2}S.
Crystals
Our highquality bulk single crystals of SnBSTS were grown by the VBT^{24}, a typical crystal boule is shown in Fig. 2a. The perfection of the grown crystals was established by Xray diffraction and Raman spectroscopy^{34,35,36} (Supplementary Figs 1 and 2, and Supplementary Notes 1 and 2, respectively). The lattice parameters (Supplementary Table 1), obtained by the refinement of Xray diffraction pattern of a powder specimen, are in agreement with tetradymite crystal phase. We observed no indication of Sn precipitates in these crystals, even at the nanoscale in our STM studies (described below), consistent with expectations from the very small Sn content used and the successful use of Sn as a resonant level dopant in small percentages in previous studies on tetradymites (see, for example, refs 24, 25, 33). The excellent cleavage characteristics of our single crystals are further indication of the absence of Sn precipitates.
Bulk transport characterization
The temperaturedependent bulk resistivity (ρ) plots (Fig. 2b) of three samples of SnBSTS from a 15cmlong single crystal boule, separated by a total of ∼8 cm along the boule, show that the bulk SnBSTS is highly insulating. ρ increases exponentially with decreasing T, attains maximum values (∼125 Ωcm was the largest observed) at ∼100–150 K and starts decreasing with decreasing T. This decrease, which has been observed numerous times in previous studies on tetradymitebased materials with low carrier concentrations, is widely taken as an indication that the resistivity of the insulating bulk material has been shortcircuited at low temperatures by the metallic TSS^{20,30,37,38}. The temperature at which the SSs finally dominate the bulk resistivity depends on intrinsic factors such as the exact defect concentration in the bulk crystal, and the surface and bulk carrier mobilities, and extrinsic factors such as the sample shape. These are the origin of the relatively small differences in behaviour observed here for crystals extracted from different locations in the large, single crystal boule. The point is that the same basic behaviour is seen for crystals extracted from widely varying positions, an indication of the uniformity of the defect chemistry in the large bulk single crystal. The high values of resistivity observed are excellent for a tetradymite; at T<100 K, the bulk resistivity must be substantially higher but it cannot be measured directly due to the dominance of the SS conductance. The Log ρ versus T^{−1} plots (Fig. 2c) exhibit an activated behaviour with the activation energy for transport Δ≈165 meV. This Δ is very high and is consistent with half of the bulk band gap measured by angleresolved photoemission spectroscopy (ARPES) (see below) (Δ=E_{g (transport)}/2, thus E_{g}=330 meV, E_{g(ARPES)}=350 meV), an indication of the intrinsic nature of the semiconducting SnBSTS crystals. The Hall coefficient (R_{H}) (Fig. 2d) increases with decreasing T and attains very high values (∼ −5 × 10^{4} cm^{3} C^{−1}) at low T. Some samples show a change in sign of R_{H} from positive to negative on cooling, which is typical behaviour for highly compensated bulk tetradymites (see, for example, ref. 39), and for T <150 K, all samples have negative R_{H}, indicating ntype carrier conduction. At the low T transport dominated by SSs, the bulk carrier concentrations must actually be substantially lower than the ∼3 × 10^{14} cm^{−3} that results when one assumes that the conduction is from bulk states only. The feature in ρ near T∼50 K, where SS transport dominates the conductance, is reproduced in all of the crystals studied and is discussed further below.
Angleresolved photoemission spectroscopy
The lowenergy band structure of SnBSTS was investigated by ARPES and is shown in Fig. 3. The observations are consistent with what has been seen in other tetradymitebased materials and no indication of the energy levels of the 1% Sndopant states is observed. The pristine crystal surface shows conical states in the centre of the surface Brillouin zone that are linearly dispersing (Supplementary Fig. 3 and Supplementary Note 3) from the DP at ∼120 meV below the Fermi level with velocity of 4 eVÅ, forming the tiny circular electron pocket (Fig. 3a). The bands probed by ARPES were then additionally electron doped through the deposition of K atoms on the surface, pushing the chemical potential into states that are not occupied in the pristine crystals. Consistent with previous studies on tetradymites, the conical bands display no photonenergy dependence, a test of the k_{z} dependence of their energy dispersion, and therefore represent SSs. The photon and kdependent ARPES spectra of the Kdeposited crystals enabled the determination of the extrema of the bulk valence and conduction bands that form the energy gap in which the SSs reside, Fig. 3b. The DP was thus found to be isolated from the bulk bands, as the highest BVB states only reach energies of 120 meV below while the lowest energy BCB states appear 230 meV above the DP (these could also be BCBderived quantum well states of electrons trapped near the surface by band bending; however, as no Rashba splitting is observed, it is likely to be that the band bending is small, and that these states only trace the bottom of the BCB^{40,41}). These findings are shown schematically in Fig. 3c. The bulk gap is found to be ∼350 meV, consistent with the transport activation energy. E_{F} falls in the SSs only and the Fermi surface, shown in Fig. 3g, consists only of a small ring centred at the Γ point of the Brillouin zone (Fig. 3f), with the Fermi wave vector k_{F}=0.03 Å^{−1}, for the SS electrons. Constant energy cuts through the band structure (Fig. 3g–i) show that the SSs, as one moves away from the DP, acquire some hexagonal warping and are joined by the six petals of the BVBs some 240 meV below the Fermi level in the pristine sample, or the circular bottom of the BCB when the chemical potential is raised by 110 meV through K deposition (Fig. 3d,e). This is confirmed in our tunnelling microscopy experiments.
Scanning tunnelling microscopy
The topographic image of the Teterminated (001) surface of an SnBSTS crystal at 30 K displays large atomically flat regions with atomic modulations corresponding to the rhombohedral crystal structure (Fig. 4a); the Fourier transform of this image reflects the hexagonal symmetry of the crystal surface (Fig. 4b). In addition to the Te atoms, several defects are observed^{26}. We probed the electronic structure on the surface of SnBSTS by using scanning tunnelling spectroscopy (STS)^{42,43,44,45}. First, we measured the differential conductance, which is proportional to the local density of states, across the surface along a line of length of 90 nm (Fig. 4c). The spectra show a ‘U’ shape curve with a minimum at −120 meV and multiple inflection points. As STS is sensitive to both TSS and bulk bands, to correctly identify the features in the spectra, the STS results are compared with the E–k structure established by ARPES. We identify the observed changes in the STS spectra at around −200 meV and +120 meV, to be the indication of the edges of the bulk bands. The tunnelling between these energies is dominated by the SSs. The minimum of the conductance corresponds approximately to the DP energy. The DP energy (120 meV below the Fermi energy) is in agreement with the ARPES data measured in different crystals from the same boule, showing the longrange homogeneity of the material. The variation in the position of the minimum energy along the scan line is small (with 2.4 meV s.d.), which suggests that the chemical potential is homogeneous at the nanometer length scale and the DP energy is not affected significantly by the defects on the surface. However, as the energy is tuned away from the DP energy, the density of states develops significant modulations. These inhomogeneities in the spectra are mainly the result of the disordered Sb–Bi distribution in the layers, which leads to enhanced quasiparticle interference on the surface. Scattering of the surface electronic states was examined by recording differential conductance maps at various energies (Fig. 4d). Although the conductance maps are strongly influenced by the SbBi disorder, the Fourier transforms of the maps capture the signal corresponding to the scattering of TSS and reveal a linearly dispersing scattering cone between the BCB and BVB (Fig. 4e). To compare the STM and ARPES data, we note that scattering between the opposite sides of the Dirac cone is prohibited by timereversal symmetry. In the case of a single Dirac cone, the prohibition suppresses the amplitude of the largest scattering wave vectors backscattering, resulting in a scattering cone with a smaller diameter. However, unambiguously resolving the diameter change is beyond our measurement resolution. Thus, we simply approximate the observed scattering cone as a manifold of vectors connecting regions of large density of states measured by ARPES. In this picture, the boundary of the observed energymomentum structure for a single linear dispersing band has half of the slope as measured by ARPES. The expected energy–momentum relation is indicated as a red line (Fig. 4e), in good agreement with our ARPES measurement.
Magnetoresistance and 2D SSs
To study the availability of the TSS for charge transport experiments and potential applications of SnBSTS in advanced devices, we performed transport measurements on crystals at 20 mK, under magnetic fields up to 18 T. Figure 5a,b are the magnetoresistance (MR) (ρ_{xx} versus H) and Hall (ρ_{yx} versus H) plots, respectively, measured by tilting H in the x–z plane (z is the direction of the surface normal and x is the direction of current flow in the basal plane). The ρ_{yx} versus H plots show that the charge transport is mainly due to electrons. Both ρ_{xx} and ρ_{yx} exhibit strong quantum oscillations at θ=90°, which gradually die out as θ approaches 0°. To visualize the oscillations and study their origin, the angular dependence of ρ_{xx} and ρ_{yx} are plotted as a function of H^{−1} (Fig. 5c,d). The Shubnikovde Haas oscillations are extracted from ρ_{xx} and ρ_{yx}, and the resulting difference resistivity (Δρ) plots are shown in Fig. 6a,b; the oscillations are as large as ∼6%, with a low frequency. For a particular oscillation peak (n=5) the field value corresponding to the peak position ((μ_{0}H)^{−1}_{n=5}) is plotted with tilt angle (Fig. 6c). It is clear that the peak shift is proportional to sinθ, which has been widely taken as a reflection of the 2D TSS origin of the oscillations (see, for example, refs 16, 18). The Fermi surface crosssection area (S_{F}) is calculated as 37 T. The 2D SS carrier density n_{s} is 8.93 × 10^{11} cm^{−2} and the SS carriers are ntype. Using the ARPES Fermi velocity (v_{F}=4eVÅ), the Fermi surface in this crystal is found to be 134 meV above the DP, consistent with ARPES and STM measurements, again an indication of the homogeneity of the material over macroscopic distances in the single crystal. (For more clarity concerning the 2D nature of the states, ρ_{xx} and ρ_{yx} are plotted as a function of (μ_{0}Hsinθ)^{−1} in Supplementary Fig. 4; the consistent shift of the peak positions of oscillations confirms that these oscillations are owing to 2D conduction (Supplementary Note 4).) We note that quantum oscillations due to the SSs are seen for the vast majority of samples that we have cut from the crystal boules of SnBSTS. Although to the authors’ knowledge there has been no systematic study of when such oscillations are present in tetradymites and when they are absent, their presence must be related to the crystal surface quality, otherwise they would be observed more frequently.
The TI crystals can be considered as having parallel conductance paths, with the measured electrical conductance being a sum of bulk (G_{bulk}) and surface (G_{s}) conductances, G=G_{bulk}+G_{s} (ref. 39). With this in mind, the SnBSTS crystals allow for the SS conductance to be characterized over a wide temperature range. Taking the data for a very high bulk resistivity crystal, G is plotted versus T^{−1} in Fig. 6d. At high T, G_{bulk} is dominant; it decreases exponentially as T decreases and for a wide range of temperatures, in the range of 150–100 K, both surface and bulk carriers are contributing significantly to the observed transport. For temperature below 100 K, surface carriers probably dominate the transport. G_{s} can then be estimated at low temperature, where the influence of the bulk is less significant. The estimated T dependence of G_{s} in the range 4–100 K is plotted in the inset of Fig. 6d. G_{s} shows an unusual step at ∼50 K. This feature may either be an experimental artefact or purely due to TSS behaviour, or due to a structural phase transition in the underlying bulk crystal. Synchrotron diffraction analysis at low T (Supplementary Fig. 5 and Supplementary Note 5) rules out the possibility of a bulk structural phase transition and the STM images taken at low T do not show any sign of a surface reconstruction. Therefore, this anomaly cannot reflect the presence of structural transitions either on the surface or in the bulk material. We speculate that it may reflect the sensitivity of conductance of TSS on SnBSTS to the adsorption of a residual active gas (for example, H_{2} or O_{2}) in the experimental chamber.
Discussion
We have shown that highly bulk insulating TI crystals of Bi_{1.08}Sn_{0.02}Sb_{0.9}Te_{2}S, with intrinsic semiconductor characteristics (Δ ∼165 meV and bulk carrier density n<3 × 10^{−14} cm^{−3} at low temperatures) can be successfully grown by the VBT, with nearly uniform properties over 8 cm or more of a large single crystal boule. The bulk band gap is consistently estimated to be ∼350 meV by spectroscopy and transport methods, and the DP is found to be completely exposed in the gap, ∼120 meV above the valence band maximum and ∼230 meV below the conduction band minimum. The chemical potential for these crystals consistently falls in the SSs only, at an energy of ∼120 meV above the DP. Quantum oscillations from the TSS electrons are reproducibly observed. The SS carriers in SnBSTS are ntype, which are preferable for charge transport experiments and potential spintronics applications. Our results lead us to conclude that SnBSTS is an excellent tetradymitetype bulk single crystal TI, and that it will be highly advantageous for use in future experimental studies of TSSs, especially for the characterization of SS quantum transport very close to the DP.
Methods
Crystal growth
The bulk single crystals were grown by the VBT. The required amounts (according to the formula: Bi_{1.08}Sn_{0.02}Sb_{0.9}Te_{2}S) of elements with high purities (5 N) were placed in carboncoated, bottompointed quartz ampoules with an inner diameter of 4 mm. The asreceived highpurity starting materials (Bi, Sb and Te) were further purified by heating under vacuum of∼10^{−5} mbar at 950 °C in the presence of carbon, in sealed quartz tubes. The crystal growth ampoules were sealed under a vacuum of∼10^{−5} mbar. The crystal growth was performed at ∼700 °C with a translation rate of ampoule of 1 mm h^{−1} through the crystallization zone^{24} and ∼15cmlong crystal boules were obtained.
Crystalline quality
The crystals extracted from the single crystal boule were studied for phase identification on a laboratory Xray diffractometer (Bruker Eco D8 Advance) equipped with CuKα source and LYNXEYE XE detector. To check the homogeneity of the crystal structure we also performed Raman microscopy at ambient temperature using 10 μW from a 532nm excitation laser, focused to 1 μm spot. Temperaturedependent synchrotron powder Xray diffraction measurements were performed on beamline 11BM at the Advanced Photon Source, to probe the bulk crystal structure at low temperature.
Bulk resistivity and carrier density
The bulk resistivity and carrier density were measured respectively in fourprobe and Hall configurations on a Quantum Design Physical Properties Measurement System. Samples were in the rectangular shape with thickness of ∼0.5 mm. The electrical contacts were made on the (001) surface through Pt wires with silver paint. The Hall data were recorded by applying magnetic field of 1 T normal to the (001) sample surface and the current flow was in the basal plane.
ARPES and STM band structure analysis
The electronic band structure was established by ARPES using a Scienta SES3000 electron spectrometer set to the resolution of 12 meV and 0.1° at beamline 12.0.1 of the Advanced Light Source. Photon energies were in the range of 30–100 eV. Samples were cleaved at 15 K in ultrahigh vacuum of 5 × 10^{−9} Pa and all the data were collected at 15 K. The STM measurements were performed on the (001) crystal surface in the temperature range of 30–90 K, on a homebuilt variable temperature STM.
MR and Hall effect
Angulardependent MR and Hall data were obtained in a dilution refrigerator at T=20 mK at applied fields up to μ_{0}H=18 T, using standard six contact measurements. The Shubnikovde Haas quantum oscillations were obtained by subtracting the background from the data. The thickness of samples used for measurements was ∼50 μm.
Additional information
How to cite this article: Kushwaha, S. K. et al. Sndoped Bi_{1.1}Sb_{0.9}Te_{2}S bulk crystal topological insulator with excellent properties. Nat. Commun. 7:11456 doi: 10.1038/ncomms11456 (2016).
References
Bernevig, B. A., Hughes, T. L. & Zhang, S.C. Quantum spin Hall effect and topological phase transition in HgTe quantum wells. Science 314, 1757–1761 (2006).
König, M. et al. Quantum spin Hall insulator state in HgTe quantum wells. Science 318, 766–770 (2007).
Kane, C. L. & Mele, E. J. Quantum spin Hall effect in graphene. Phys. Rev. Lett. 95, 226801 (2005).
Fu, L., Kane, C. L. & Mele, J. Topological insulators in three dimensions. Phys. Rev. Lett. 98, 106803 (2007).
Xia, Y. et al. Observation of a largegap topologicalinsulator class with a single Dirac cone on the surface. Nat. Phys. 5, 398–402 (2009).
Moore, J. E. & Balents, L. Topological invariants of timereversalinvariant band structures. Phys. Rev. B 75, 121306(R) (2007).
Xu, Y. et al. Observation of topological surface state quantum Hall effect in an intrinsic threedimensional topological insulator. Nat. Phys. 10, 956–963 (2014).
Wei, P. et al. Exchangecouplinginduced symmetry breaking in topological insulators. Phys. Rev. Lett. 110, 186807 (2013).
Vobornik, I. et al. Magnetic proximity effect as a pathway to spintronic applications of topological insulators. Nano Lett. 11, 4079–4082 (2011).
Chang, C.Z. et al. Highprecision realization of robust quantum anomalous Hall state in a hard ferromagnetic topological insulator. Nat. Mater. 14, 473–477 (2015).
Fu, L. & Kane, C. L. Probing neutral Majorana fermion edge modes with charge transport. Phys. Rev. Lett. 102, 216403 (2009).
Akhmerov, A. R., Nilson, J. & Beenakker, C. W. J. Electrically detected interferometry of Majorana fermions in a topological insulator. Phys. Rev. Lett. 102, 216404 (2009).
Seradjeh, B., Moore, J. E. & Franz, M. Exciton condensation and charge fractionalization in a topological insulator Film. Phys. Rev. Lett. 103, 066402 (2009).
Hsieh, D. et al. A tunable topological insulator in the spin helical Dirac transport regime. Nature 460, 1101–1105 (2009).
Analytis, J. G. et al. Twodimensional surface state in the quantum limit of a topological insulator. Nat. Phys. 6, 960–964 (2010).
Checkelsky, J. G., Hor, Y. S., Liu, M.H., Cava, R. J. & Ong, N. P. Quantum interference in macroscopic crystals of nonmetallic Bi2Se3 . Phys. Rev. Lett. 103, 246601 (2009).
Chen, Y. L. et al. Experimental realization of a threedimensional topological insulator, Bi2Te3 . Science 325, 178–181 (2009).
Qu, D.X., Hor, Y. S., Xiong, J., Cava, R. J. & Ong, N. P. Quantum oscillations and Hall anomaly of surface states in the topological insulator Bi2Te3 . Science 329, 821–824 (2010).
Xu, S.Y. et al. Discovery of several large families of topological insulator classes with backscatteringsuppressed spinpolarized singleDiraccone on the surface. Preprint at http://arxiv.org/abs/1007.5111 (2010).
Ren, Z., Taskin, A. A., Sasaki, S., Segawa, K. & Ando, Y. Large bulk resistivity and surface quantum oscillations in the topological insulator Bi2Te2Se. Phys. Rev. B 82, 241306(R) (2010).
Ji, H. et al. Bi2Te1.6S1.4: A topological insulator in the tetradymite family. Phys. Rev. B 85, 201103(R) (2012).
Hasan, M. Z. & Kane, C. L. Colloquium: topological insulators. Rev. Mod. Phys. 82, 3045–3067 (2010).
Zhang, H. et al. Topological insulators in Bi2Se3, Bi2Te3 and Sb2Te3 with a single Dirac cone on the surface. Nat. Phys. 5, 438–442 (2009).
Kushwaha, S. K. et al. Comparison of Sndoped and nonstoichiometric verticalBridgmangrown crystals of the topological insulator Bi2Te2Se. J. Appl. Phys. 115, 143708–143713 (2014).
Ren, Z., Taskin, A. A., Sasaki, S., Segawa, K. & Ando, Y. Fermi level tuning and a large activation gap achieved in the topological insulator Bi2Te2Se by Sn doping. Phys. Rev. B 85, 155301 (2012).
Jia, S. et al. Defects and high bulk resistivities in the Birich tetradymite topological insulator Bi2+xTe2xSe. Phys. Rev. B 86, 165119 (2012).
Jia, S. et al. Lowcarrierconcentration crystals of the topological insulator Bi2Te2Se. Phys. Rev. B 84, 235206 (2011).
Arakane, T. et al. Tunable Dirac cone in the topological insulator Bi2xSbxTe3ySey . Nat. Commun. 3, 636 (2012).
Pan, Y. et al. Low carrier concentration crystals of the topological insulator Bi2−xSbxTe3−ySey: a magnetotransport study. New J. Phys. 16, 123035–123050 (2014).
Ren, Z., Taskin, A. A., Sasakai, S., Segawa, K. & Ando, Y. Optimizing Bi2xSbxTe3ySey solid solutions to approach the intrinsic topological insulator regime. Phys. Rev. B 84, 165311 (2011).
Teramoto, I. & Takayanagi, S. Relations between the electronic properties and the chemical bonding of SbxBi2xTe3ySey system. J. Phys. Chem. Solids 19, 124–129 (1961).
Pauling, L. The formula, structure and chemical bonding of tetradymite, Bi14Te13S8, and the phase Bi14Te15S6 . Am. Mineral. 60, 994–997 (1975).
Christopher, M. J., Kulbachinskii, V. & Joseph, P. H. Resonant level formed by tin in Bi2Te3 and the enhancement of roomtemperature thermoelectric power. Phys. Rev. B 80, 233201 (2009).
Neumann, G. & Seideġġer, R. Über die existenz verschiedener phasen im quasibinären system Bi2Se2  Bi2S3 . Helv. Phys. Acta 40, 293–300 (1967).
Richter, W. & Becker, C. R. A Raman and farinfrared investigation of phonons in the rhombohedral V2–VI3 compounds Bi2Te3, Bi2Se3, Sb2Te3 and Bi2(Te1−xSex)3 (0<x<1), (Bi1−ySby)2Te3 (0<y<1). Phys. Stat. Solid. (B) 84, 619–628 (1977).
Zhao, S. Y. F. et al. Fabrication and characterization of topological insulator Bi2Se3 nanocrystals. Appl. Phys. Lett. 98, 141911–141913 (2011).
Xiong, J. et al. Quantum oscillations in a topological insulator Bi2Te2Se with large bulk resistivity (6 Ω cm). Phys. E 44, 917–920 (2012).
Taskin, A. A., Ren, Z., Sasaki, S., Segawa, K. & Ando, Y. Observation of Dirac holes and electrons in a topological insulator. Phys. Rev. Lett. 107, 016801 (2011).
Xiong, J. et al. High field Shubnikovde Haas oscillations in the topological insulator Bi2Te2Se. Phys. Rev. B 86, 045314 (2012).
Bahramy, M. S. et al. Emergent quantum confinement at topological insulator surfaces. Nat. Commun. 3, 1159 (2012).
Bianchi, M. S. et al. Coexistence of the topological state and a twodimensional electron gas on the surface of Bi2Se3 . Nat. Commun. 1, 128 (2010).
Roushan, P. et al. Topological surface states protected from backscattering by chiral spin texture. Nature 460, 1106–1109 (2009).
Seo, J. et al. Transmission of topological surface states through surface barriers. Nature 466, 343–346 (2010).
Beidenkopf, H. et al. Spatial fluctuations of helical Dirac fermions on the surface of topological insulators. Nat. Phys. 7, 939–943 (2011).
Gyenis, A. et al. Quasiparticle interference on the surface of the topological crystalline insulator. Phys. Rev. B 88, 125414 (2013).
Acknowledgements
This research was supported by the ARO MURI on TIs, grant W911NF1210461, ARO grant W911NF1210461 and the MRSEC programme at the Princeton Center for Complex Materials, grant NSFDMR1420541. The ARPES experiments were performed under the LBNL and BNL grants DEAC0205CH11231 and DESC0012704. This research used resources of the Advanced Photon Source, a U.S. Department of Energy (DOE) Office of Science User Facility operated for the DOE Office of Science by Argonne National Laboratory under Contract No. DEAC0206CH11357. The Raman experiments were conducted with support from the National Science Foundation (grant DMR1410846).
Author information
Authors and Affiliations
Contributions
S.K.K., H.J. and R.J.C. designed the research. S.K.K. synthesized the compound, performed optimized crystal growth, Xray and bulk electronic measurements. I.P. and T.V. performed ARPES studies. T.L., J.L., W.W. and N.P.O. carried out and interpreted the MR transport measurements. A.G. and A.Y. performed the lowtemperature STM measurements. Y.T., H.Z. and K.S.B. performed the Raman experiments. S.L. performed the lowtemperature Xray diffraction measurements. S.K.K. and R.J.C. wrote the manuscript with input from all the coauthors.
Corresponding authors
Ethics declarations
Competing interests
The authors declare no competing financial interests.
Supplementary information
Supplementary Information
Supplementary Figures 15, Supplementary Table 1, Supplementary Notes 15 and Supplementary References (PDF 453 kb)
Rights and permissions
This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/
About this article
Cite this article
Kushwaha, S., Pletikosić, I., Liang, T. et al. Sndoped Bi_{1.1}Sb_{0.9}Te_{2}S bulk crystal topological insulator with excellent properties. Nat Commun 7, 11456 (2016). https://doi.org/10.1038/ncomms11456
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/ncomms11456
This article is cited by

Improved electrical conductivity and power factor in Sn and Se codoped meltgrown Bi2Te3 single crystal
Journal of Materials Science: Materials in Electronics (2021)

Weak Antilocalization and Anisotropic Magnetoresistance as a Probe of Surface States in Topological Bi2TexSe3−x Thin Films
Scientific Reports (2020)

Chemical instability at chalcogenide surfaces impacts chalcopyrite devices well beyond the surface
Nature Communications (2020)

Anomalous phonon softening in the topological insulator Sndoped Bi1.1Sb0.9Te2S
Science China Physics, Mechanics & Astronomy (2020)

Unusual Conductance Fluctuations and Quantum Oscillation in Mesoscopic Topological Insulator PbBi4Te7
Scientific Reports (2019)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.